A new joining-device for manufacturing tubular butt joints with higher curing temperatures of film adhesives
© The Author(s) 2017
Received: 17 August 2017
Accepted: 18 September 2017
Published: 20 September 2017
For detailed stress distribution analysis of bondlines, non-linear finite element analysis (FEA) is necessary. Depending on the load case in relation to shear and tension/compression adhesives show a different behaviour of the yield point , which is e.g. included in the Mahnken and Schlimmer  model. State of the art for biaxial tested adhesive material-characteristics is the use of bonded tubular butt joints under variable torsion and tension loads. Important for the quality of the determined material values is the alignment of both tubes. The quality is significantly improved, if both tubes are aligned perfectly coaxial. Also, the bondline has to be free of voids. In previous work , Wölper investigated the effects of coaxial and angle deviations for the results of material characteristics using FEA. A slight deviation has a strong negative impact to the results. Particularly for thin film-adhesives with elevated curing temperatures, the change of viscosity of the adhesive and the thermal expansion of the tubes must be considered. Previous investigations regarding the manufacturing of the specimens showed shortfalls in joining and curing them. Due to voids, geometric deviations or poorly-bonded tubes, no reliable results were achieved yet. Therefore, a new assembly-device is developed and tested. The results show well joined tubes without a significant angle deviation and with an average of 40 µm in coaxial deviation. The thickness of the bondline can be adjusted and is constant over the whole diameter. The new joining-device enables the testing of tubular butt joints to determine biaxial material values of thin higher-temperature-cured film-adhesives. The device is patented to DE 102017114538.9.
KeywordsAdhesive bonding Tubular butt joint Joining device Elevated curing temperature Biaxial testing
In order to use the potentials of carbon-fibre-reinforced-polymer (CFRP) as a light weight structure material, not only CFRP material characteristics are important. Further, adhesive bonding, with its good characteristics  for joining fibre reinforced plastics, leads to weight reduction. A major point of interest is the acquisition of precise material characteristics of adhesives. In order to design adhesive joints with finite element analysis (FEA) simulations, high sophisticated material models as Mahnken and Schlimmer, Drucker Prager or TAPO should be used in a continuum mechanic simulation approach. All of the models need biaxial material data. One possible solution is the use of arcan specimen . According to the literature, arcan specimens can be used, but bonded specimens require complex test assemblies and are costly in manufacturing. Tubular butt joints allow for combined tension–torsion tests overcoming the need to use different sample types for different loading conditions.
Based on experiences from first trials another approach is taken to align both tubes during cure. By clamping only one tube and guiding the other, consolidation force is applied by an additional weight on the guided adherend to provide the sufficient pressure to the adhesive. The result is an improved quality of the bondline but results in an unintentional variation of 25% in bondline thickness. Material tests of five specimens revealed a shear-strengths variation of 20% and a variation of ultimate shear strain of 27%.
In a study, Wölper  described the effects of geometrical deviations to the stress distribution within the bondline of hollow tubular butt joints by using non-linear elasto-plastic FEA simulation. According to test regulations,  the coaxial deviation of an outer tube with a diameter of 60 mm has to be smaller than 0.06 mm. Wölper identified strength critical stress peaks at the free edge of bondline beginning with deviations of 0.05 mm under torsion loading.
Homogeneous bondline thickness
Coaxial deviation smaller than 0.05 mm
Angle deviation smaller than 0.031°
No air inclusion or voids in the bondline
The aim of the presented joining concept is to increase the specimen quality whereby the variance of test results should decrease. A new concept for joining the tubes is developed and presented.
Materials and experimental methods
To prevent a gap between both tubes due to an axially thermal expansion, the core has to be divided into two parts. A male and a female part of the core result which have a small loose fit to each other, minimising the coaxial tolerances. Being the same material with the same thermal expansion, the bearing persists over the entire temperature range of the cure cycle. The core has a sealing element to prevent an excessive adhesive flow from the bondline to the core. An outer sealing of the bondline is realised by a heat resistant tape. With a weight on top of the tubes, a consolidation force is applied to the bondline to prevent any voids and air inclusions.
Calculation of design parameters
Labels of variables used in Eq. (2)
Diameter of core
Inner diameter of tube
Thermal expansion coefficient of core material
Thermal expansion coefficient of tube material
Start cure temperature of adhesive
The diameter Dc of the core at environmental temperature can be calculated by Eq. 2. The sealing diameter can be calculated by changing the thermal expansion coefficient αC to the sealing value αS. The higher temperature Tcur,s is set to the temperature Tv where the viscosity of the adhesive falls below 1000 Pa s. A squeeze out of adhesive needs to be prevented.
Selection of materials
Thermal coefficient of expansion (1/K)
Temperature of onset (°C)
Diameter at 23 °C (mm)
16 ∙ 10−6
130 ∙ 10−6
260 ∙ 10−6
Hysol® EA9695 is used as film adhesive for the bonding. Differential scanning calorimetry (DSC) analysis identifies the onset of cure at 120 °C and the highest curing rate at 130 °C. Measurements reveal the point of lowest viscosity of 1000 Pa s is at 90 °C  for EA 9695.
Results and discussion
The calculated curve shows the temperature of the middle diameter of the tubes.
Surface preparation and alignment of tubes
First, the bonding surfaces of the tubes are cleaned by acetone and isopropanol, then pre-treated by abrasive blasting with corundum F220 (0.05–0.07 mm, 2 bar) as described in . After blasting, the tips are cleaned a second time in acetone and isopropanol bath and ventilated in an oven at 23 °C for 20 min.
Measured coaxial and angle deviations of 20 bonded specimen
To ensure the quality of the bondline in homogeneous thickness, exclusion of voids or air, the specimen are cut and polished for microscopy. An average bondline thickness is measured to 40 µm all over the bondline at three bar pressure during manufacturing.
Present test results
As the project is still in progress, only 20 of 200 specimens are tested at the moment. Available results show a variation of 5.35% in maximum shear strength. In comparison to the literature , the absolute tested shear strength is 18% higher.
Manufacturing trials show an excellent joining device for hollow tubular butt joints with reproducible properties. The concept with the smaller diameters of the core and sealing enable an easy to use joining of the components. The parameters which influence the specimen’s quality, only depend on the manufacturing quality of the male and female core. All manufactured specimen are free of voids and air inclusion and show the same bondline thickness. With 0.04 mm the bondline is at its minimum thickness guaranteed by an integrated polyvinyle carrier fleece. Typically wide bonded plates bonded with the adhesive show a thickness of 0.1 mm. With the small wall thickness of 3 mm of the tubes, the adhesive leaks out till the carrying-fleece of the film adhesive is fully compressed. A possible solution is the stacking of additional adhesive layers. If the bondline thickness does not depend on the carrying fleece, another outer sealing concept needs to be used.
The coaxial and angular deviations are statistical smaller than the test regulations. To guarantee a proper basis for FEA input data  more tests need to be done.
From the present test results, the variation of material values decreased by a factor 4. But there is no information about the maximum strain of the specimens in test. All variables with negative impact to the test results are mitigated. The new concept allows testing of film adhesives with elevated curing temperatures in tubular butt joints and ensures high quality material data.
A new concept for manufacturing tubular butt joint specimens for biaxial film adhesive material characteristics is presented. While the different thermal expansions are the main problem for manufacturing tubular butt joints with film adhesives in the past, the presented new joining concept utilizes these to align both adherends during the curing. The quality of bondline and the accuracy of orientation of the tubes are strongly increased. At this time the material tests show a decrease of variation in results of factor 4. The joining device is registered to Patent Number DE 102017114538.9.
Further investigations have to ensure the adjustment of the bondline thickness by varying the number of adhesive film layers. Otherwise the concept must to be redesigned to comply with this requirement. Hollow tubular butt joints are now cheap to manufacture and provide a high quality and a low variation of test data for different loading states in one type of specimen.
MJS, JKo, DHo and CHu are the developer of the named patent. TLo supported with surface pre-treatment before bonding. All authors read and approved the final manuscript.
The authors thank the German Ministry of Commerce for the funding of the FACTOR project. DLR thanks the FhG. IFAM for testing the specimen.
The authors declare that they have no competing interests.
Availability of data and materials
Consent for publication
Ethics approval and consent to participate
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Bornemann J, Schlimmer M. Berechnungen und Auslegung von Klebverbindungen (Teil 2). Adhaes Kleb Dicht. 2004;48:40–2. doi:10.1007/BF03251309.Google Scholar
- Mahnken R, Schlimmer M. Simulation of strength difference in elasto-plasticity for adhesive materials. Int J Numer Methods Eng. 2005;63:1461–77. doi:10.1002/nme.1315.View ArticleGoogle Scholar
- Wölper J, Löbel T, Kosmann J. Usability of tube torsion/tension test for determination of film adhesive material properties. Conference report. AB2015 Porto, Portugal, 2–3 July 2015. 2015.Google Scholar
- Habenicht G. Kleben–erfolgreich und fehlerfrei, vol. 6. Berlin: Vieweg + Teubner; 2012. p. 2–3. doi:10.1007/978-3-8348-8316-2.Google Scholar
- Cognard J, Cèac’hcadec R, Sohier L, Davies P. Analysis of the nonlinear behavior of adhesives in bonded assemblies—Comparison of TAST and Arcan tests. Int J Adhes Adhes. 2008;28:393–404. doi:10.1016/j.ijadhadh.2008.04.006.View ArticleGoogle Scholar
- Henkel, Hysol EA 9695. Epoxy film adhesive technical report. Henkel Corporation, Rev.1/01. 2017.Google Scholar
- DIN EN 14869-1. Structural adhesives-determination of shear behaviour of structural bonds—Part 1: Torsion test method using butt-bonded hollow cylinders German version. Germany. 2011.Google Scholar
- Badey J, Espuche E, Jugnet Y, Chabert B, Duc Tran Minh. Influence of chemical and plasma treatments on the adhesive properties of PTFE with an epoxy resin. Int J Adhes Adhes. 1996;16:173–8. doi:10.1016/0143-7496(95)00042-9.View ArticleGoogle Scholar
- KELUX Kunststoffe GmbH. Eigenschaften PTFE-material datasheet, Germany. 2016.Google Scholar
- DEW-Stahl. Werkstoffdatenblatt 1.4305-material datasheet, Germany. 2017.Google Scholar
- Silicone I. Technische Daten und Verarbeitungshinweise-material datasheed, Germany. 2016.Google Scholar
- Löbel T. The Hybrid bondline: a novel disbond-stopping design for adhesively bonded composite joints. Dissertation, Technische Universität Braunschweig, Germany. 2016.Google Scholar
- ISO 17212. Structural adhesives-guidelines for the surface preparation of metals and plastics prior to adhesives bonding, Switzerland. 2012.Google Scholar
- Tomblin J et al. Shear stress-strain data for structural adhesives, Federal Aviation Administration, USA DOT/FAA/AR-02/97. 2002.Google Scholar